{'fraction_non_alphanumeric': 0.03948143783146729, 'fraction_numerical': 0.01767825574543312, 'mean_word_length': 4.875432525951557, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Facile synthesis of CNT interconnected PVP-ZIF-8 derived hierarchically porous Zn/N co-doped carbon frameworks for oxygen reduction.

In this work, a strategy has been adopted to construct an architecture through the coordination of polyvinylpyrrolidone (PVP) and a monodisperse zeolitic imidazolate framework (ZIF-8), which was entwined by carbon nanotubes (CNTs) firstly, followed by a pyrolysis process to obtain the hybrid catalyst. The meticulous design of the hybrid material using CNTs to interconnect the PVP assisted ZIF-8 derived porous carbon frameworks together produces a hierarchical pore structure and dual-heteroatom (Zn/N) doping (Zn-N/PC@CNT). Without further acid treatment, the hybrid material prepared after pyrolysis at 900 °C (PVP-ZIF-8@CNT-900) has been demonstrated as an efficient non-precious metal catalyst for the oxygen reduction reaction (ORR) with its superior stability compared to the commercial 20 wt% Pt/C catalyst in alkaline media. The catalyst shows better performance towards the ORR, with its more positive onset and half-wave potentials (Eonset = 0.960 V vs. RHE and E1/2 = 0.795 V vs. RHE) than the counterpart system which is free of both CNT and PVP. The high performance of the hybrid catalyst can be ascribed to the co-existence of dual-active sites with hierarchical pore structures originating from the synergistic effects between Zn/N co-doped porous carbon and CNTs. We further demonstrated the single-cell performance by using the homemade system as the cathode catalyst for the Alkaline Exchange Membrane Fuel Cell (AEMFC) system, which showed a maximum power density of 45 mW cm-2 compared to 60 mW cm-2 obtained from the 40 wt% Pt/C catalyst.